REV. CHIM. (Bucureti) 60 Nr. 1 2009
Conservation-restoration of Textile Materialsfrom Romanian Medieval Art Collections
I. Spectral characteristics of the naturally aged silk
OCTAVIANA MARINCA1, MARIA GIURGINCA2*1 George Enescu University of Arts, 189 Srrie Str, 700451, Iai, Romania2 Politehnica University, Faculty of Material Science and Engineering, 1 Gh. Polizu Str., 011061, Bucharest, Romania
The most representative pieces belonging to the thesaurus-collection of Putna Monastery most of themdonations from the part of Prince Stephan the Great and the Holly have been selected. Some of thesecultural heritage objects are dated, while others have been only written down in the documents of their time(XVth XVIth centuries). Analysis and characterization of the micro-samples taken over for experiments aimat elucidating of the mechanisms of natural ageing. To this end, the micro-samples have been analysed byFTIR spectrometry, for the identification of the materials and of their extent of damage. The destructive,hydrolysis and denaturation type processes have been evidenced by the spectral characteristics specificto amides I and II, and also to the hydroxylic groups. An important observation was that the samples takenover from objects with pronounced functional wear and tear have suffered processes of hydrolysis anddenaturation of the polypeptidic chain. A correlation has been established between the degradation of thepolypeptidic chain and the manner in which the object had been utilized.
Keywords: textile materials, IR spectral analysis, natural ageing, silk
Fig. 1. Cultural heritage objectsconsidered for the study:
a cover for tomb;b Catasarghion; c iconostasisveil Crucifixion; d deacon stole
The medieval art collections organized in Romania inthe second half of the XXth century contain unique objectsof inestimable artistic value. Most of these textile treasures,gathering an important number of pieces, have beenpreserved along the centuries by the Orthodox Church inits monasteries, known as having played an especiallyimportant part over the whole history of our nation. Theconstant concern for their safe preservation andtransmission from generation to generation necessarilyinvolves a scientific approach both from a historical artisticperspective and equally from a practical one, namely theirconservation and possible restoration.
Investigations on the historical textiles may contributeto create an as faithful as possible image with therespective epoch.
At present, the researches devoted to the physico-chemical characterisation of the textile materials from oldart collections are scarce; generally, only an approximate,descriptive visual analysis being made. .
Recent studies on the characterisation and conservationassessment of the cultural heritage objects are based oncomplex investigation systems, among which specialmention should be made of: special photographictechniques, radiographic techniques, IR spectroscopy, UV Vis absorption spectrometr y, chromatographictechniques, differential thermal and thermogravimetricanalyses, X ray fluorescence, mass spectrometry,microscopic techniques [2-9].
Considering all the above-mentioned aspects, thepresent paper is devoted to the scientific investigation of
the historical textile materials from the collection ofRomanian medieval art treasured at Putna Monastery, thedistrict of Suceava.
Experimental partSilk samples, taken over from various cultural heritage
textile goods, have been employed for IR spectralcharacterization.
MaterialsFrom the art collection of Putna Monastery, micro-
samples, the codes and significance of which are listed intable 1, have been taken over.
Figure 1 illustrates the textile objects considered for thestudy.
EquipmentFTIR spectrometer, Jasco (Japan) (4000 400 cm-1
domain)Reactives: Spectral potassium bromide (Merck,
Germany) for inclusion of the suitable broken up fibers
Results and discussionsAnalysis and characterization of the micro-samples
permitted a correlation between the conservationcondition and the results of the investigations, for betterunderstanding of the mechanisms governing the processof natural ageing.
* Tel.: 021 315 41 93
REV. CHIM. (Bucureti) 60 Nr.1 2009
Table 1MICRO-SAMPLES TAKEN OVER FROMCULTURAL HERITAGE OBJECTS OF
Table 2SPECTRAL CHARACTERISTICS OF NATURAL SILK
All samples have been qualitatively characterized forthe identification of the type of material used by artisanswho weaved or embroidered the objects, comparativelywith the traditional materials (silk, cotton, hemp) viewedas reference.
Spectral characteristics of the reference sampleNatural silk is a proteic fibre, mainly including in its
structure the following amino-acids: glycine, alanine, serineand tyrosine, with -arrangement quite close to that ofpolyglycine, and an identity period of 7.0 , which indicatesa slight wrinkle, as due to the inter and intra molecularhydrogen bonds among chains. The polypeptidic chainsare constituted of units of the RCH-CO-NH- type,
connected head to head, and differing among them bythe nature of the R radical from the lateral chain.
On the basis of such general information, the main bandsoccurring in the IR spectrum of a natural silk referencesample have been assigned. The characteristics bands andtheir assignment in the IR spectrum (fig. 2) of natural silkare presented in table 2.
Consequently, in the 3450 3050 cm-1 domain, the NHgroup evidences characteristic bands, attributed to thevalency vibration of the NH and OH groups, both associatedand non-associated through hydrogen bonds. The aspectof the bands from 3420 and 3306 cm-1 indicates anadvanced association among chains, the higher intensityof the band from 3306 cm-1 representing also acharacteristic of the wrinkled conformation [10-12].
REV. CHIM. (Bucureti) 60 Nr. 1 2009
Fig 2. IR spectrum of reference silk
Fig. 3. IR spectra of the micro samples under analysis
The carbonyl group (C = O) generates typical vibrationsat 1707 cm-1 (valency vibration) and at 1650 cm-1 (amideI). The band from 1707 cm-1 is a low intensity one, probablyresulting from a marginal acid rest.
The NH group evidences deformation vibrations at 1530cm-1 similar to those of the secondary amides (amide II),as well as rocking-type vibrations ( NH) over the 675 420 cm-1 domain, included together with those of the CH2groups, and attributed to the whole skeleton.
The CH, CH2 and CH3 alkyllic groups, of bothasymmetrical and symmetrical type, show valencevibrations over the 3000 2800 cm-1 domain.
The band from 1230 cm-1 is attributed to the C-N structurefrom the skeleton of the polypeptide .
Characterisation of the silk samples from Putna collectionThe IR spectral analysis of the silk samples taken over
from Putna collection was performed in the sameconditions applied for the reference. The spectra obtainedare plotted in figure 3.
Examination of the spectra showed that the main bandsare similar to those of the reference. However, certaindifferences were noticed in the aspect of the bands from3420 and 3300 cm-1, namely three different situationsof the ratio in which they occur, as follows:
-a higher intensity of the band from 3420 cm-1 (P2-AV,P4-CR, P4-CA, P5BG, P5-DR, P6A, P9FV), indicating thepresence of some structures with NH groups, partiallyassociated through hydrogen bonds, which may be dueeither to the breaking of some transversal bonds alongchains, as result of some slow destructive processes, or toa treatment in which the molecule had adopted thepreponderantly extended configuration, with the marginalNH group
-a higher intensity of the band from 3300 cm-1 (P3AFG,P3ATV, P9FV), indicating an association through inter- andintramolecular hydrogen bonds 
-an equal intensity of the two absorption bands (P7-B,P8R, P9AM), indicating the simultaneous presence of thetwo types of structures, associated through transversalhydrogen bands in different ways.
Also, some low intensity additional bands may occur inthe 1550 1670 cm-1 region, as due to the succession ofsome aminoacids with certain structural peculiarities inthe macromolecule; it is the case of some samples (P2_AR,P2_AG, P5_BRF, P6_V) not considered in the present study,whose additional bands from 1670 and 1570 cm-1 mightresult from an aromatic group present in tyrosine and / orphenylalanine.
The polypeptidic chain of silk suffers a degradationprocess during its processing, utilization and prolongedstoring, induced by physicochemical (light, temperature,humidity, atmospheric pollutants), biological andmicrobiological (bacteria fungi, microorganisms) factorswhich contribute to the occurrence of certain structuralmodifications.
In the case of cultural heritage objects, all suchmodifications are produced over long periods of time,being part into evidence by spectral data.
The transformation of the polypeptidic chain resultsfrom processes of oxidation, hydrolysis and / ordenaturation of the amidic structure.
Knowledge of the main spectral characteristics of silkfrom the IR domain permitted selection of a few bandsthat might turn to good account the structural modificationproduced during degradation.
Thus, in the IR domain, there have been considered thebands from 1650 1630 cm-1 (amide I) and 1550 1530cm-1 (amide II), as well as the wide band from 3450 3300cm-1 ( OH + NH), and the distance between the twoamidic structures ( = AI - AII). There have been alsofollowed the evolution of the band from 1230 cm-1 (amideIII), responsible for the CN + NH vibrations producedin the main chain.
Knowing the absorbency value of ea